|Year : 2014 | Volume
| Issue : 3 | Page : 132-136
Physicochemical characterization: Comparative evaluation of three allograft biomaterials and autogenous bone
Antoine Berberi1, Antoine Samarani2, Nabih Nader1, Rita Mearawi1, Wasfi Kanj1, Bassam Badran2
1 Department of Oral And Maxillofacial Surgery, School of Dentistry, Lebanese University, Lebanon
2 Ecole Doctorale, Prase, Lebanese University, Lebanon
|Date of Web Publication||8-Dec-2014|
Department of Oral And Maxillofacial Surgery, School of Dentistry, Lebanese University, Lebanon
Source of Support: This project was supported by a grant from the
EcoleDoctorale, Lebanese University, Conflict of Interest: None
Objectives: Bone substitutes (BSs) used in oral surgery include allografts, xenografts, and synthetic materials that are frequently used to compensate bone loss or to reinforce repaired bone by encouraging new bone in growth into the defect site. The aim of this study was to evaluate a number of physical and chemical properties in a variety of allografts biomaterials used in oral surgery and to compare them with those of autogenous bone. Materials and Methods: Autogenous bone and three different allograft biomaterials were studied by high-resolution X-ray diffractometry (XRD), atomic absorption spectrometry, laser diffraction, and checked for their chemical composition, calcium release concentration, crystallinity, and granulation size. Results: The highest calcium release concentration was 24.94 mg/g for Puros ® and the lowest one was 4.05 mg/g for OsteoSponge ® compared to 20.15 mg/g to natural bone. The range of particles size, in term of median size D 50 , varied between 630.47 μm for Puros ® and 902.41μm for OsteoSponge, ® compared to 282.1μm for natural bone. Bone and Puros ® displayed a hexagonal shape as bone except and OsteoSponge ® which showed a triclinic shape. Conclusion: A BS of choice depends largely on its clinical application that is associated to its biological and mechanical performance. These morphological differences between biomaterials greatly influence their in vivo behavior of biomaterials. Significant differences were detected in terms of calcium concentration, particles size, and crystallinity.
Keywords: Allograft, bone, calcium concentration, granulometry, X-ray diffraction
|How to cite this article:|
Berberi A, Samarani A, Nader N, Mearawi R, Kanj W, Badran B. Physicochemical characterization: Comparative evaluation of three allograft biomaterials and autogenous bone. J Dent Res Rev 2014;1:132-6
|How to cite this URL:|
Berberi A, Samarani A, Nader N, Mearawi R, Kanj W, Badran B. Physicochemical characterization: Comparative evaluation of three allograft biomaterials and autogenous bone. J Dent Res Rev [serial online] 2014 [cited 2023 Jan 30];1:132-6. Available from: https://www.jdrr.org/text.asp?2014/1/3/132/146491
| Introduction|| |
Bone is a living tissue that serves structural support and calcium metabolism. Bone matrix is organic and consists of a network of collagen protein fibers impregnated with mineral salts (85% of calcium phosphate, 10% of calcium carbonate, and 5% of calcium fluoride and magnesium fluoride). The mineral compartment of bone is predominantly present in the form of calcium hydroxyapatites (Ca 10 [PO 4 ] 6 [OH] 2 ). Bone tissue also contains negligible quantities of non-collagen proteins, including the family of bone morphogenetic proteins (BMPs). 
Calcium plays an important role on osteoconductivity and on enhanced bone tissue integration via entrapment and concentration of circulating bone growth factors (BMPs) and osteoprogenitor cells, thus imparting osteoinductive properties of these materials. , The effect of calcium ions on bone tissue response has been investigated in several in vivo as well as in vitro studies, where Ca-incorporated titanium implant were shown to enhance osseintegration. ,,,
Bone tissue serves as a reservoir and a source of calcium for metabolic needs through the process of bone remodeling. The role of phosphate in bone development also should not be over looked since bone maintains body's pH balance by producing additional carbonates and phosphates. First phosphorus is laid down during the mineralization process, and then calcium binds to it. ,
Autogenous bone is osteogenic (cells within a donor graft synthesize new bone at implantation sites), osteoinductive (new bone is formed by active recruitment of host mesenchymal stem cells from surrounding tissue, which differentiate into bone-forming osteoblasts), osteoconductive (vascularization and new bone formation into the transplant), and highly biocompatible. , This process is facilitated by the presence of growth factors within the autogenous bone material (mainly BMPs).  These characteristics should be present in an idealsubstitute and all bone grafting materials canbe classified according to these characteristics. 
The greatest success in bone grafting has been achieved with autogeneous bone ("gold standard"), fulfilling all essential physicochemical and biological properties, despite its inherent limitations as availability and postoperative pain. ,[13 ],,,,,,,,,
Numerous biomaterials have been successfully used as BS, such as allografts (human), xenografts (porcine or bovine), and synthetic calcium-based materials (β-tricalcium phosphate (β-TCP) and hydroxyapatite (HA)), and a combination of these with or without the use of membrane and screws. ,,,,,
Allografts do not have the drawbacks of autografts, but are less successful in clinical practice. ,,,
Ideally, a BSshould be osteoconductive, providing three-dimensional scaffolds for growth of vessels and osteoprogenitor cells. Finally, it should be resorbable.
Moreover, resorption rate should match the formation rate of new bone tissue.  In fact; while, a too fast degradation of the biomaterial can exert negative effect on bone regeneration processes,  the presence of BS residual grafted particles after bone healing may lead to formation of a "composite repair tissue" rather than to a regenerated bone tissue. 
The aim of this study was to evaluate some of physical and chemical properties in a variety of commercially available allograft biomaterials that are frequently used for dental applications as BS and to compare them with autogenous bone.
| Materials and Methods|| |
A total of three commercially available allograft BS were included in this study (Puros ® , OsteoSponge ® , and DynaBlast™ ).
Each material was used with the lowest particle size range available. Analytical methods were used to investigate these properties, techniques such as atomic absorption spectrometry (AAS), laser diffraction (LD), and X-ray diffractometry (XRD). AAS was used to determine concentration of calcium ion in BS, LD was used to measure granulate size, and XRD to identify phase and composition features and qualitatively evaluate crystallinity of materials. Comparisons of the properties of the commercial products with the properties of autogenous bone were also explored.
The following data were taken from the manufacturer's specifications. All samples were obtained directlyfrom manufacturers in sealed vials and used without further treatment.
DynaBlast™ (Keystone Dental, Inc, 144 Middlesex Tumpike Burlington, MA 01803, USA) is a combination of human tissue (tissue banks in the USA) that has been demineralized and cancellous bone mixed with poloxamer reverse phase resorbable medium and formulated into a paste or putty-like form. 
Puros ® (Zimmer Dental Inc, 1900 Aston Ave. Carlsbad, CA 92008, USA) is an allogeneic graft material treated by Tutoplast ® process that gently removes unwanted material such as fat, cells, antigens, and inactivates pathogens; while preserving the valuable minerals and collagen matrix. It is available as cortical granulate, particle size 0.25-2 mm. ,
OsteoSponge ® (Bacterin International Inc, 600 Cruiser Lane Belgrdae, MT 59714 USA) allograft consists of 100% of demineralized human cancellous bone, with no additional carrier materials. OsteoSponge ® is prepared using methods that preserve native growth factors.  The granulate size varies between 1 and 4 mm.
The bone samples were collected during mandibular third molars surgery (gamma-irradiated), rinsed with ethanol, dried in vacuum at room temperature, and ground in agate mortar. ,
Calcium and phosphorous release from graft material in demineralized water was evaluated using AAS (WFX-210, RayLeigh, BRAIC, China). For this aim, standards for calcium and phosphorous within the range between 0.5 and 10 µg/L were prepared. 0.4mg of each biomaterial (all nine sample) was immersed in100mL of 0.9% NaCland the pH was adjusted at 7 by using hydrochloric acid (0.1N). The variation of Ca concentration was determined at D 0 (day 0), D 2 (day 2), and each week after, until the week 6. The concentration was calculated based on the Beer-Lambert law. 
LD for particle size measurement
Particle size distribution was determined using a laser scattering particle size analyzer (Patrica LA-950 V2 Horiba Instruments, Japan). The measurement method relies on the basis of Mie scattering theory, with measuring range varying between 0.01 and 3 μm using an ultrasonic probe with measuring time of 20s at a frequency of 20 kHz. The devise is equipped with an optical system of two light sources, a laser diode of approximately 1.6 mW with λ = 650 nm and a 405nm light-emitting diode of approximately 0.3 mW. Large particles scatter light at small angles relative to the laser beam and small particles scatter light at large angles. The particle size is reported as a volume equivalent sphere diameter. , Samples were well mixed and homogenized in their powder state prior to their analysis. Average particle size and distribution were calculated for all nine biomaterials studied and autogenous bone.
In order to determine the crystal phases in the explored biomaterials, X-ray powder diffract meter was used. Homogenized powder samples (2-3 g) were compressed in PVC lenses (diameter 2.5 cm, thickness 2 mm) and measured using a D8 Bruker diffract meter (copper anticathode λ Ka =0.154060 nm). Range of 2θ between x° and y° was chosen to obtain maximum information about crystal phases. Collected diffract grams were analyzed by the software EVA (Bruker Corporation, Billerica, Massachusetts, USA) based on powder diffraction files provided by the International Center for Diffraction Data (ICDD). Crystallite size analysis was calculated using the peak broadening of XRD reflection that is used to estimate the crystallite size (in an orthogonal direction to the crystal plane) using the following formula: 
Where, X sis the crystallite size in nanometer, λ is the wavelength of X-ray beam in nanometer (λ =0.15406nm in our case), and FWHM is the full width at half maximum for the diffraction angle at 2θ =25.9° that was selected according to (002) Miller's plane family).
| Results|| |
AAS results of calcium concentration over the observation period are showed in [Table 1].
|Table 1: The calcium concentration as derived from AAS experiments by brand names and time period |
Click here to view
OsteoSponge ® revealed the lowest calcium release concentration (4.05 mg/g) followed by DynaBlast™ (6.2 mg/g). The calcium concentration of Puros ® (24.94 mg/g) was comparable to autogenous bone (20.15 mg/g).
The particles median size D 50 (in volume percentages), the particle size range expressed by the 10 and 90 percentiles (D 10 and D 90 , respectively) and the particles size ranges reported by the manufacturers as determined by the LD measurements are all presented in [Table 2].
Results showed that Puros ® had the lowest median particle size (630.47 μm) followed by DynaBlast™ (777.14 μm), while OsetoSponge ® had the highest one (902.41μm).
No one shows a median size close to the one ofautogenous bone (282.1 μm). The narrowest size distribution was observed with BioOss ® (0.26-8.92μm) followed byIngenios™β-TCP (3.90-15.18 μm). The widest size distribution was observed with OsteoSponge ® (174.62-2,301.84 μm) followed by DynaBlast™ (39.24-1,754.62 μm) and Puros ® (174.62-1,167.72 μm).
The results of the XRD experiments that are indicative for the chemical composition of the BS are shown in [Table 3] except for DynaBlast™ as the material is presented in putty paste form and not granulate one. These materials diffract more and less the X-ray, which means diverse degrees of crystallinity, as indicated in the different peaks widths [Figure 1].
|Figure 1: X-ray diffraction data for all investigated samples. All data were measured at. 1.54 Å as wavelength and the displayed range in 2Ø was chosen to optimally represent the relevant features|
Click here to view
|Table 3: Chemical compositions and shapes of samples as derived from X - ray diffractometry except for DynaBlast® (presented in putty paste from) |
Click here to view
The common crystal phase was calcium phosphate silicate hydroxide (Ca 5 (PO 4 ) 2.85 (SiO 4 ) 0.15 (OH)) and autogenous bone.
Except for OsteoSponge ® samples were crystallized at different levels of crystallinity in hexagonal systems. The OsteoSponge ® sample is the only sample crystallized in triclinic system.
| Discussion|| |
The more higher the calcium concentration, more are the biomaterials prone to degradation. ,, The acidic buffer, to some extent, mimics the acidic environment during osteoclastic activity or bone resorption. ,, In vivo biodegradability can be achieved by dissolution or cell-mediated, multinuclear cells; osteoclasts; and macrophages are involved in phagocytosis. ,,,,
In our study, different allograft biomaterials had different calcium releasing. This could be explained by the fact that the speed of biodegradability of BS, in vivo or in vitro, depends on their composition, particle size, crystallinity, porosity, and preparation. ,,,,
From the particle size related data, it can be concluded that, in general, size ranges measured for tested materials were different from those reported by manufacturers who do not specify the used technique in the crystalline material's characterization and could explain the noticed differences. [40 ],,,, However, it should be kept in mind that the granules under analysis differed not only in their size but also in their physicochemical properties.
The influence of properties and characteristics of BS on biological response cannot be easily predicted as the published studies involve different types of BS in different particle size ranges. Regarding the ranges of particle size that were tested in the present investigation, there was no relation between the sizes of particles and calcium concentration with the time.
XRD diffractograms of various materials, including human bone, were quite similar with common crystal phase calcium phosphate silicate hydroxide (Ca 5 (PO 4 ) 2.85 (SiO 4 )0.15 (OH). However, silicates, when they are present, are not major components of the crystal phases, since their stoichiometry compared to phosphate (2.85) are considerably negligible (0.15). It must be highlighted that in bone and all BS Ca to P ratios are fluctuating between 1.75 and 1.33. This could mean that calcium is the major element that compensates phosphate charges.
XRD diffractograms showed that all samples, including natural bone, proved to have the same anisotropic crystal size (9.42Ε in a and b-directions and 6.8Ε in c-direction with alpha and beta 90° and gamma 120°), OsteoSponge ® showed different anisotropic size 6.2Ε in a and 11.9Ε in b-directions and 5.6Ε in c-direction with alpha and beta 97° and gamma 120°; 6.25Ε in a-direction, 11.9 Ε in b-direction, and 5.6 Ε in c-direction with alpha 97 and beta 114° and gamma 93°, respectively.
Theseresults demonstrated that crystal shape of Puros ® and autogenous bone are similar, hexagonal shape, and OsteoSponge ® showed a triclinic shape. This structure is the poorest system in the symmetric properties.
| Conclusions|| |
Three different allograft materials were herein investigated, and results were compared to autogenous bone. Even when similar chemical characteristics were found, significant differences were detected in terms of calcium concentrations, particles size, and crystallinity. Although these morphological differences greatly influence in vivo behavior of the biomaterial, they are often not taken into consideration when the samples' biological performance is evaluated. It is believed that results provided for biomaterials investigated will be most useful to fully understand their clinical behavior and response. Since, the BS of choice depends largely on the possible clinical application and its associated biological and mechanical needs, it is important not to assume that all BS will show the same pattern of performance and that the validation of a BS in one clinical site may not necessarily predict its identical performance in another anatomical location. Hopefully in the future, hybrid or complex combination products that include cells, growth factors, and/or gene therapy in combination will be likely to provide oral surgeons more effective tools for bone defects reparation. In this regard, it is obvious that further studies are warranted.
| Acknowledgments|| |
The authors would like to thank Manal Houhou, Sarah Hadda, Sahar Rihan, and Hussein Bassal for their excellent technical assistance.
| References|| |
Kay MI, Young RA, Posner AS. Crystal structure of hydroxyapatite. Nature 1964;204:1050-2.
Ripamonti U, Klar RM. Regenerative frontiers in craniofacial reconstruction: Grand challenges and opportunities for the mammalian transforming growth factor-β proteins. Front Physiol 2010;11:143.
LeGeros RZ. Calcium phosphate-based osteoinductive materials. Chem Rev 2008;108:4742-53.
Hanawa T, Kamiura Y, Yamamoto S, Kohgo T, Amemiya A, Ukai H, et al
. Early bone formation around calcium-ion-implanted titanium inserted into rat tibia. J Biomed Mater Res 1997;36:131-6.
Sul YT, Byon ES, Joeng Y. Biomechanical measurements of calcium-incorporated oxidized implants in rabbit bone: Effect of calcium surface chemistry of a novel implant. Clin Implant Dent Relat Res 2004;6:101-10.
6. Fröjd V, Franke-Stenport V, Meirelles L, Wennerberg A. Increased bone contact to a calcium-incorporated oxidized commercially pure titanium implant: An in-vivo
study in rabbits. Int J Oral Maxillofac Surg 2008;37:561-6.
Kang BS, Sul YT, Johansson CB, Oh SJ, Albrektsson T. The effect of calcium ion concentration on the bone response to oxidized titanium implants. Clin Oral Implant Res 2014;23:690-97.
Orimo H. The mechanism of mineralization and the role of alkaline phosphatase in health and disease. J Nippon Med Sch 2010;77:4-12.
Reddi AH. Role of morphogenetic proteins in skeletal tissue engineering and regeneration. Nat Biotechnol 1998;16:247-52.
Kenley RA, Yim K, Abrams J, Ron E, Turek T, Marden LJ, et al
. Biotechnology and bone graft substitutes. Pharm Res 1993;10:1393-401.
Block MS, Kent JN. Sinus augmentation for dental implants: The use of autogenous bone. J Oral Maxillofac Surg 1997;55:1281-6.
Wheeler SL. Sinus augmentation for dental implants: The use of alloplastic materials. J Oral Maxillofac Surg 1997;55:1287-93.
Greenwald AS, Boden SD, Goldberg VM, Khan Y, Laurencin CT, Rosier RN. American Academy of Orthopaedic Surgeons. The Committee on Biological Implants. Bone-graft substitutes: Facts, fictions, and applications. J Bone Joint Surg Am 2001;83:98-103.
Parikh SN. Bone graft substitutes: Past, present, future. J Postgrad Med 2002;48:142-8.
Finkemeier CG. Bone grafting and bone-graft substitutes. J Bone Joint Surg Am 2002;84-A: 454-64.
Sandor GK, Lindholm TC, Clokie CM. Bone regeneration of the cranio-maxillofacial and dento-alveolar skeletons in the framework of tissue engineering. In: Ashammakhi N, Ferretti P, editors. Topics in Tissue Engineering. Ch 7. 2003. p. 1-46.
Ben-Nissan B. Natural bioceramics: From coral to bone and beyond. Curr Opin Solid State Mater Sci 2003;7:283-8.
Vallet-Regi M, Gonzales-Calbet JM. Calcium phosphate as substitution of bone tissues. Prog Solid State Chem 2004;32:1-31.
Hing KA, Wilson LF, Buckland T. Comparative performance of three ceramic bone graft substitutes. Spine J 2007;7:475-90.
Rueger JM, Linhart W, Sommerfeldt D. Biologic reactions to calcium phosphate ceramic implantations. Results of animal experiments. Orthopade 1998;27:89-95.
Bohner M. Calcium orthophosphates in medicine: From ceramics to calcium phosphate cements. Injury 2000;31:37-47.
Bohner M. Physical and chemical aspects of calcium phosphates used in spinal surgery. Eur Spine J 2001;10:114-21.
Bouchlariotou I, Bernard JP, Carrel JP, Vazquez L. Long-term stability of osseointegrated implants in bone regenerated with a collagen membrane in combination with a deproteinized bovine bone graft: 5-year follow-up of 20 implants. POSEIDO 2013;1:45-53.
Toeroek R, Dohan Ehrenfest DM. The concept of Screw-Guided Bone Regeneration (S-GBR). Part 3: Fast Screw-Guided Bone Regeneration (FS-GBR) in the severely resorbed preimplant posterior mandible using allograft and Leukocyte- and Platelet-Rich Fibrin (L-PRF): A 4-year follow-up. POSEIDO 2013;2:93-100.
Toeroek R, Dohan Ehrenfest DM. The concept of Screw-Guided Bone Regeneration (S-GBR). Part 2: S-GBR in the severely resorbed preimplant posterior mandible using bone xenograft and Leukocyte- and Platelet-Rich Fibrin (L-PRF): A 5-year follow-up. POSEIDO 2013;2:85-92.
Sung HJ, Meredith C, Johnson C, Galis ZS. The effect of scaffold degradation rate on three-dimensional cell growth and angiogenesis. Biomaterials 2004;25:5735-42.
Glowacki J. A review of osteoinductive testing methods and sterilization processes for demineralized bone. Cell Tissue Bank 2005;6:3-12.
Moore ST, Katz JM, Zhukauskas RM, Hernandez RM, Lewis CS, Supronowicz PR, et al
. Osteoconductivity and osteoinductivity of Puros (R) DBM putty. J Biomater Appl 2011;26:151-71.
Traini T, Piatelli A, Caputi S, Degidi M, Mangano C, Scarano A, et al
. Regeneration of human bone using different bone substitute biomaterials. Clin Implant Dent Relat Res 2013.
Klein CP, Driessen AA, de Groot K, van den Hooff A. Biodegradation behavior of various calcium phosphate materials in bone tissue. J Biomed Mater Res 1983;17:769-84.
Irinakis T. Efficacy of injectable demineralized bone matrix as graft material during sinus elevation surgery with simultaneous implant placement in the posterior maxilla: Clinical evaluation of 49 sinuses. J Oral Maxillofac Surg 2011;69:134-41
Schmitt CM, Doering H, Schmidt T, Lutz R, Neukam FW, Schlegel KA. Histological results after maxillary sinus augmentation with Straumann® BoneCeramic, Bio-Oss®, Puros®, and autologous bone. A randomized controlled clinical trial. Clin Oral Implants Res 2013;24:576-85.
Peters F, Scwarz K, Epple M. The structure of bone studied with synchroton X-ray diffraction, X-ray absorption spectroscopy and thermal analysis. Thermochim Acta 2000;361:131-8.
Figueiredo M, Henriques J, Martins G, Guerra F, Judas F, Figueiredo H. Physicochemical characterization of biomaterials commonly used in dentistry as bone substitutes-comparison with human bone. J Biomed Mater Res B Appl Biomater 2010;92:409-19.
García R, Báez AP. Atomic Absorption Spectrometry (AAS), Atomic Absorption Spectroscopy. In: Dr. Farrukh MA, editor. Ch. 1. InTech; 2012. p. 1-13.
Markoviæ S, Veselinoviæ L, Lukiæ MJ, Karanoviæ L, Braèko I, Ignjatoviæ N, et al
. Synthetical bone-like and biological hydroxyapatites: A comparative study of crystal structure and morphology. Biomed Mater 2011;6:45-50.
Tadic D, Epple M. A thorough physicochemical characterisation of 14-calcium phosphate-based bone substitution materials in comparison to natural bone. Biomaterials 2004;25:987-94.
Harold KP, Leroy EA. X-Ray Diffraction Procedures: For Polycrystalline and Amorphous Materials. In: Klug HP, Leroy EA, editor. 2 nd
ed. New York: Wiley-Interscience; 1974. p. 992.
Hannink G, Arts JJ. Bioresorbability, porosity and mechanical strength of bone substitutes: What is optimal for bone regeneration? Injury 2011;42 Suppl 2:22-5.
Bacterin, product information on Osteosponge ®
, 2014. Available from: http://www.bacterin.com/products/osteospoge [Last accessed on 2014 Aug 29].
Zimmer dental, products, regenerative, bone grafts, information on Puros ®
, 2014. Available from: http://www.zimmerdental.com/revamp2k5/regenerative [Last accessed on 2014 Aug 29].
KeyStone Dental Inc. product information on DynaBlast™
, 2014. Available from: http://www.keystonedental.com/products/dynablast [Last accessed on 2014 Aug 29].
Gschneidner K, Pecharsky V, Tsokol A. Recent developments in magnetocaloric materials. Rep Prog Phys 2005;68:1479-539.
Chesnick IE, Fowler CB, Mason JT, Potter K. Novel mineral contrast agent for magnetic resonance studies of bone implants grown on a chick chorioallantoic membrane. Magn Reson Imaging 2011;29:1244-54.
[Table 1], [Table 2], [Table 3]